A SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST

 Suzan Barrett
 4 months ago
 Views:
Transcription
1 A SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST P. Robinson The Composites Centre, Department of Aeronautics, Imperial College London South Kensington, London, SW7 2AZ, UK SUMMARY This paper reports on the development of a Mode I interlaminar test which has been designed to indicate the crack position on the loaddisplacement curve so avoiding the requirement to monitor the crack length during the test. Results of the selfindicating test show good agreement with the conventional Mode I test method. Keywords: Mode I, delamination, toughness INTRODUCTION The double cantilever beam (DCB) specimen, shown in Figure 1, has become the established specimen for the measurement of delamination toughness of composites in Mode I [1,2]. applied load, P A A opening displacement, δ initial crack length, a 0 midplane section AA: delamination film laminated zone Figure 1: Conventional DCB specimen The usual test procedure is to record force (P), displacement (δ) and crack length (a) as the delamination advances. A data reduction technique based on beam theory or compliance calibration is then applied to calculate the Mode I critical energy release rate, G Ic. A disadvantage of the DCB specimen is that the crack length measurement is usually obtained by visual observation of one edge and as a consequence the results can vary according to the skills of the person conducting the test. Even if the test operator is
2 experienced the development a skewed crack front due to material variability or, in the case of woven composite specimens, the presence of multiple cracks due to disbonding of transverse yarns can lead to very uncertain measurement of crack lengths. It is possible to determine G Ic without using the measured crack length but then the formula for G Ic relies on an analytical expression for the specimen stiffness which itself may not be an accurate representation of the actual specimen behaviour. Another solution to the crack length problem is to avoid visual observation by using crack length gauges or other sensors attached to the specimen [3] but these can add expense and complexity to the test set up. This paper explores a simple modification to the conventional DCB test specimen to make visual observation of the crack length unnecessary. DEVELOPMENT OF THE APPROACH The basis of the approach is to modify the specimen so that the crack length can be inferred from the loaddisplacement curve recorded in a test and to use the area method to determine G Ic. The specimen is modified by altering the starter delamination film. In the conventional test specimen this film is incorporated at the midplane of the laminate to provide the initial, or starter, delamination (Fig. 1). Various modified forms of the delamination film have been considered and some are shown in Figure 2. The initial growth in a specimen using pattern (a) is stable but as the crack front approaches the right hand edge of the first laminated rectangular zone the crack growth becomes unstable and the crack will arrest after partial growth into the next laminated zone. The unstable growth means that data reduction using the area method is not valid. a) delamination film laminated zones b) delamination film laminated zones c) delamination film laminated zones Figure 2: Modified delamination patterns An alternative pattern of delamination film, which will ensure stable crack growth, is shown in Figure 2b. Here the crack front initially advances through a laminated zone of constant width in a stable manner and, assuming that G Ic remains constant, the load will be steadily reducing. When a step increase in laminated zone width is encountered the crack growth will arrest and an increase in load will be recorded on the load
3 displacement plot until crack growth restarts in the wider laminated zone. The energy consumed as the crack grows from the start to the end of one of the constant width laminated zones can be determined and hence, using the area of the zone, G Ic can be calculated. It is important that the steps in the laminated width are sufficiently large to cause a suitably distinct change in the loaddisplacement curve and with this in mind the possible number of steps in laminated zone width will be limited by the width of the specimen for the pattern of Figure 2b. This limitation can be overcome by using a pattern of the type shown in Figure 2c in which, between the step changes, the width of the laminated zone steadily reduces with crack length though clearly there is the potential for unstable growth in the tapered width zones. This pattern is the basis of the selfindicating Mode I toughness specimen which is explored in this paper. ANALYSIS AND DESIGN OF THE SELFINDICATING SPECIMEN This section analyses the geometry influence on the crack growth stability for the pattern of Figure 2c and describes the pattern design used in the test programme. Stability analysis Figure 3 defines the geometry of the initial part of the selfindicating starter delamination pattern with the crack front having advanced a distance (aa 1 *) into the first laminated zone where a is the distance to the crack front and a 1 * is the distance to the start of the first laminated zone, both measured from the load line. l 2 a l 1 crack front B B 1 w delamination film laminated zones loading line a 1 * a 2 * a 3 * a 1 a 2 a 3 Figure 3: Geometry of the selfindicating pattern The energy release rate at the crack front is given by = 2 (1) in which P is the applied load, w is the width of the delamination crack front and C is the compliance (i.e. δ/p). To cause crack growth P must be sufficiently large to ensure = (2)
4 For crack growth to be stable the following condition must be satisfied < (3) and if G Ic is assumed to be constant then this condition becomes <0 (4) Treating each arm of the specimen as a cantilever which is builtin across the full width of the specimen at the crack front, the arm compliance from simple beam theory is = 2 3 (5) where E is the longitudinal Young s modulus of the arm material and I is the 2 nd moment of area of the arm cross section. Replacing P in equation 1 as δ/c and substituting for C using equation 5 then the condition for stable crack growth (equation 4) can be shown to be satisfied for a displacementcontrolled test providing the crack length meets the following condition: < (6) in which l 1 is length of the triangle of which that laminated zone forms part. Equation 6 defines the criterion for stability for crack growth in the initial laminated zone of the pattern of Figure 3. Equation 6 can be also applied to crack growth in the subsequent laminated zones; for the i th laminated zone a 1 * and l 1 are replaced by the values of a i * and of l i. Specimen design To simplify the design of the selfindicating specimen, the values of l i and a i (the length of the i th laminated zone) are set to constant values, l and a respectively, and by choosing the starting width of each laminated zone to be equal to that of the first zone (i.e. B 1 ) then the areas of the laminated zones are all equal. To ensure stable growth up to the end of the i th laminated zone there must be sufficient laminated material beyond the end of this zone to ensure that the builtin assumption is still reasonable and the following condition on the length of each laminated zone must be satisfied. < 4 +4 (7) An additional condition, which is important in the specimen design, concerns the step increase in laminated width at the junctions between consecutive laminated zones. The load, P init, required to initiate crack growth in the next laminated zone is related to the
5 load, P arr, at crack arrest at the end of the previous laminated zone, according to simple beam theory, by the following equation. h = h (8) Equation 8 can be used to ensure that there is a sufficiently distinct change in the loaddisplacement curve during the crackarrest phase between consecutive laminated zones. Table 1 gives the geometry of the selfindicating specimen designed using equations 7 and 8 for the experimental evaluation. Table 1: Dimensions of the selfindicating specimen No. of laminated zones a* (mm) a (mm) l (mm) B (mm) B 1 (mm) EVALUATION OF THE SELFINDICATING APPROACH Manufacturing details Three types of specimen were prepared (see Fig. 4). These were selfindicating specimens, conventional DCB specimens (to provide a G Ic value for comparison with that measured with the self indicating specimens) and specimens containing a single triangular shaped laminated zone (to assess the accuracy of the stability criterion of equation 6). loading line Triangle A Triangle B Conventional DCB 20 Selfindicating Figure 4: Geometry of the test specimens (dimensions in mm) Materials All specimens were manufactured from panels of unidirectional carbon epoxy laminate laid up using a Hexcel prepreg (914CT3006K). To produce the required starter
6 delamination pattern a 12.5 µm Teflon film was incorporated at the midplane of the laminate. All laminates were 330 mm (fibre direction) x 300 mm and consisted of 24 plies giving a nominal cured thickness of 3 mm. Preparation and insertion of delamination pattern To reduce the effect of any variation in G Ic between laminates or within a laminate, the three different types of specimens were interspersed as uniformly as was practical across the prepared laminates. Therefore a fairly complex delamination starter pattern of the type shown in Figure 5 had to be cut and positioned within the prepreg assembly. The pattern included small cutouts along the outer edges which are used to correctly cut the specimens from the cured panel. prepreg panel Teflon film cutouts Figure 5: Example of starter delamination pattern To prepare the film, a fullscale drawing of the required delamination pattern was printed and taped to cardboard on a flat working surface. A transparent sheet of Melinex film (0.05mm thick) was taped over the drawing and the Teflon delamination film was placed on top of the Melinex. The Teflon layer adhered naturally to the Melinex due to static electricity and did not need to be taped to hold it in position. A scalpel and ruler were then used to cut the required pattern along the lines of the pattern drawing which was visible through the film layers. Care was taken not to cut completely through the Melinex layer as much as possible. Once the pattern had been completely cut, all the loose pieces of Teflon film were removed (i.e. in the positions that would form the laminated zones). The backing film was removed from one face of a 12 ply prepreg assembly and the exposed face was positioned carefully onto the Teflon film. The tape securing Melinex was then cut and the Melinex, Teflon and prepreg assembly was then inverted and the Melinex carefully peeled away from the Teflon layer which was left adhered to the surface of the prepreg.
7 Another 12ply pregreg assembly was then positioned on top of the film to complete the layup. Curing and preparation of specimens The laminates were cured in accordance with the manufacturer s recommendations but omitting the postcure procedure. One surface of each panel was marked out with strips of approximately 5 mm width along the edges of the panel and perpendicular to these strips two to three short lines, to be used as alignment guides, were marked along each edge across the strip width into the interior of the panel. These strips were then cut from the edge of the panel and each strip was separated at its midplane to locate the cutouts (see Fig. 5). The position of the cutouts were measured relative to the alignment lines and were marked on the edge of the remainder of the panel. From the original cutting pattern drawing the positions of all the specimens could then be marked out and the specimens machined from the panel. Specimen preparation was completed by adhesively bonding aluminum loading blocks at the loading end of each specimen and marking a scale along one edge of each conventional DCB specimen for monitoring the crack growth. Test Procedure The specimens were tested in a 100 kn Instron test frame fitted with a 500 N load cell. The tests were conducted at a crosshead displacement speed of 2 mm/minute and during each test load and crosshead displacement data were recorded by computer. For the conventional DCB test a CCD camera was used to enable a greatly magnified image of the crack tip zone on one edge of the specimen to be observed on a monitor. As the crack reached each crack length increment an event marker signal was recorded with the associated load and displacement data. In the case of the conventional DCB specimen the crack was grown by 50mm before the test was halted and the specimen unloaded. The tests of the selfindicating specimens were stopped after the crack growth had passed through the final specially shaped laminated zone. For the triangle delamination pattern specimens each specimen was tested until the crack growth became unstable and the fracture surface was then examined by eye to determine the location of the transition from stable to unstable growth. Results Loaddisplacement data The conventional DCB specimens showed the characteristic steady reduction in load as the crack advanced. For the selfindicating specimens, the typical loaddisplacement curve is shown in Figure 6. This plot clearly shows the increase in load which occurs in when the crack front reaches a stepchange in the laminated zone width. The plot also shows a steady reduction in load as the crack advances through each laminated zone indicating that the crack growth was stable as intended. The triangle delamination specimens all showed an initial steady reduction in applied load as the crack grew and a sharp drop in load when the crack growth became unstable. The crack length, a crit, at onset of the unstable growth is presented in Table 2 together with the predicted value according to equation 6. The actual crack length at the onset of
8 unstable growth exceeded the theoretical prediction by approximately 10mm for all the specimens. Figure 6: Typical loaddisplacement plot for the selfindicating specimens Table 2: Crack length at onset of unstable growth in Triangle specimens a Specimen type crit (mm) (see Fig. 4) Experiment A B Experiment average Theory (eq. 6) Data Reduction The modified beam theory data reduction scheme [1,2] was used to determine G Ic from the conventional DCB test data. As indicated earlier, the area method was used for the selfindicating specimens. The energy consumed, U i, as the crack advanced from the start of the i th laminated zone to the next (see Fig. 7) was determined from the loaddisplacement data as = in which P i and δ i are the load and displacement at the maximum of the loaddisplacement curve associated with the start of the i th laminated zone. The value of G Ic was then calculated by dividing U i by the area, A lam,i, of the i th laminated zone. In the (9)
9 selfindicating specimens used here the area of the laminated zones was constant, A lam, and so the value of G Ic was given by = (10) (P i, δ i ) (P i+1, δ i+1 ) P U i δ Figure 7: Calculation of energy consumed for selfindicating specimen A MATLAB program was written to locate the maximum associated with the start of each laminated zone, to numerically evaluate the integral of equation 9 and, finally, to calculate G Ic according to equation 10. G Ic results The mode I interlaminar toughness measured with the conventional DCB specimen displayed a slight rising Rcurve as shown in Figure 8. The average toughness measured in five specimens rose from approximately 0.11 kj/m 2 at initiation to approximately 0.13 kj/m 2 at the end of the 50mm of crack growth. The scatter of data at a particular crack length was generally contained within a band of ±0.005 kj/m 2. The data from the selfindicating tests are shown in Figure 8 where for each laminated zone the average value of G Ic of all five specimens tested is plotted as a line over the crack length range associated with that laminated zone. The range of toughnesses for a given laminated zone was typically ±0.015 kj/m 2 which is rather larger than that observed in the DCB specimens for a given crack length. The toughness measured in the first laminated zone is higher than from the conventional DCB test but this may be because the crack front profile varies during the test. The crack front shape at the first peak in the loaddisplacement trace (associated with initiation of growth) is unlikely to be identical to the shape at the next peak (associated with the junction of adjacent laminated zones) and so the area swept through by the crack front between the first two peaks may not be equal to A lam. It can be observed that the G Ic value measured in the second laminated zone is only slightly higher than the DCB values and that the rising G Ic trend in the conventional DCB specimens is also seen in the data from the selfindicating specimens.
10 G Ic (kj/m 2 ) DCB 1 DCB 2 DCB 3 DCB 4 DCB 5 self ind zone 1 self ind zone 2 self ind zone 3 self ind zone 4 self ind zone Crack length, a (mm) Figure 8: G Ic data from conventional DCB and selfindicating specimens CONCLUSIONS It has been shown that by suitably modifying the delamination film pattern in a conventional DCB specimen, the area swept out by the crack front can be inferred from distinct features on the experimental loaddisplacement trace. It is therefore possible to determine G Ic using an areabased data reduction method without direct observation of the crack length. Such an approach may be useful for woven composite laminates for which crack length observation is difficult. The data reduction procedure can be completely automated and may therefore be suitable for quality control testing. ACKNOWLEDGEMENTS The assistance of Algie Ko and Kelvin Khong in evaluating the selfindicating approach during their undergraduate projects is gratefully acknowledged. References 1. ASTM D (2007)e2. Standard Test Method for Mode I Interlaminar Fracture Toughness of Unidirectional FiberReinforced Polymer Matrix Composites 2. ISO 15024:2001. Fibrereinforced plastic composites  Determination of mode I interlaminar fracture toughness, G IC, for unidirectionally reinforced materials 3. S. Yarlagadda, A. Abu Obaid, M. K. Yoon, N. Hager, R. Domszy "An Automated Technique for Measuring Crack Propagation during Mode I DCB Testing", Society of Experimental Mechanics, X International Congress, Hilton Costa Mesa, 2004 June 710
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationApplication of fracture mechanicsbased methodologies for failure predictions in composite structures
Application of fracture mechanicsbased methodologies for failure predictions in composite structures Zoltan Mikulik a, B. Gangadhara Prusty a, Rodney S. Thomson b, Donald W. Kelly a,* a School of Mechanical
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationInterlaminar fracture characterization in composite materials by using acoustic emission
5th International Symposium on NDT in Aerospace, 1315th November 2013, Singapore Interlaminar fracture characterization in composite materials by using acoustic emission Ian SILVERSIDES 1, Ahmed MASLOUHI
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationFIS Specifications for Flex Poles (Edition May 2008) Original Text: German
FIS Specifications for Flex Poles (Edition May 2008) Original Text: German 1 Field of Application and Basic Information The following FIS specifications for flex poles are intended to ensure that flex
More informationCHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS
Oral Reference Number: ICF100942OR CHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS T. Kevin O Brien U.S. Army Research Laboratory Vehicle Technology Directorate
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationFracture Behavior. Section
Section 6 Fracture Behavior In January 1943 the oneday old Liberty Ship, SS Schenectady, had just completed successful sea trials and returned to harbor in calm cool weather when... "Without warning and
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationA PROTOCOL FOR DETERMINATION OF THE ADHESIVE FRACTURE TOUGHNESS OF FLEXIBLE LAMINATES BY PEEL TESTING: FIXED ARM AND TPEEL METHODS
1 A PROTOCOL FOR DETERMINATION OF THE ADHESIVE FRACTURE TOUGHNESS OF FLEXIBLE LAMINATES BY PEEL TESTING: FIXED ARM AND TPEEL METHODS An ESIS Protocol Revised June 2007, Nov 2010 D R Moore, J G Williams
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationThe fracture behaviour of structural adhesives under high rates of testing.
Engineering Fracture Mechanics, vol 76, 009, 868889 The fracture behaviour of structural adhesives under high rates of testing. B.R.K. Blackman, A.J. Kinloch, F.S. Rodriguez Sanchez, W.S. Teo & J.G. Williams
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More informationASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE MATERIAL
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 1617 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
More informationSTRENGTH AND STIFFNESS REDUCTION OF LARGE NOTCHED BEAMS
STRENGTH AND STIFFNESS REDUCTION OF LARGE NOTCHED BEAMS By Joseph F. Murphy 1 ABSTRACT: Four large glulam beams with notches on the tension side were tested for strength and stiffness. Using either bending
More informationEnergy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing the effect of residual stresses
International Journal of Adhesion & Adhesives 20 (1999) 59 70 International Journal of Adhesion & Adhesives Energy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationID1160 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING
ID116 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING K. Minnaar and M. Zhou = School of Mechanical Engineering Georgia Institute
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationDELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS
DELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS L Iannucci 1, M S I Shaik Dawood 1,2,3, E Greenhalgh 1 and A K Ariffin 3 1 Aeronautics Department, Imperial College London, South Kensington
More informationAcoustic emission analysis for failure identification in composite materials
Acoustic emission analysis for failure identification in composite materials Markus G. R. Sause Experimental Physics II Institute of Physics University of Augsburg 1. Motivation 2. Methods of AE analysis
More informationAPPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN
28 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES APPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN Tuyen Tran*, Dan Simkins**, Shen Hin Lim*,
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationAgnieszka Bondyra, Pawe Gotowicki
Journal of KONES Powertrain and Transport, Vol. 17, No. 1 21 INFLUENCE OF A CROSSHEAD RATE AND A NUMBER OF STRESS CYCLES ON MEASUREMENT RESULTS IN THE INPLANE SHEAR TEST FOR A CROSSPLY VINYLESTERCARBON
More informationDIGITAL IMAGE CORRELATION TECHNIQUE IN MEASURING DEFORMATION AND FAILURE OF COMPOSITE AND ADHESIVE
DIGITAL IMAGE CORRELATION TECHNIQUE IN MEASURING DEFORMATION AND FAILURE OF COMPOSITE AND ADHESIVE Ab Ghani A. F Sustainable Maintenance Engineering Research Group, Universiti Teknikal Malaysia Melaka,
More informationIMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS OBTAINED WITH LMS SAMTECH SAMCEF
V ECCOMAS Thematic Conference on the Mechanical Response of Composites COMPOSITES 015 S.R. Hallett and J.J.C. Remmers (Editors) IMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS
More informationAE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF HOOP STRESSES FOR A THINWALL PRESSURE VESSEL
Objective AE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF OOP STRESSES FOR A TINWA PRESSURE VESSE This experiment will allow you to investigate hoop and axial stress/strain relations
More informationInitiation de fissure dans les milieux fragiles  Prise en compte des contraintes résiduelles
Initiation de fissure dans les milieux fragiles  Prise en compte des contraintes résiduelles D. Leguillon Institut Jean le Rond d Alembert CNRS/UPMC Paris, France Parvizi, Garrett and Bailey experiments
More informationA New Methodology for Fiber Optic Strain Gage Measurements and its Characterization ABSTRACT
.3 A New Methodology for Fiber Optic Strain Gage Measurements and its Characterization Van Roosbroeck Jan, C. Chojetzki, J. Vlekken, E. Voet, M. Voet Fiber Optic Sensors and Sensing Systems (FOS&S), Cipalstraat
More informationA FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
TRENDS IN COMPUTATIONAL STRUCTURAL MECHANICS W.A. Wall, K.U. Bletzinger and K. Schweizerhof (Eds.) c CIMNE, Barcelona, Spain 2001 A FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
More informationDELAMINATION IN MODE I AND II OF CARBON FIBRE COMPOSITE MATERIALS : FIBRE ORIENTATION INFLUENCE
DELAMINATION IN MODE I AND II OF CARBON FIBRE COMPOSITE MATERIALS : FIBRE ORIENTATION INFLUENCE F. LACHAUD 1,2, R. PIQUET 2, L. MICHEL 1 2 LMT, IUT de énie Mécanique, 50, Chemin des Maraîchers, 31077 TOULOUSE
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationReliable Test Results
Intelligent testing Johannes J.Bührle  Agenda Reliable test results are a fundamental and highly topical aspect of materials testing. Using suitable examples we would like to show you how we view this
More informationPhysical Properties Testing Technical Bulletin
Technical Bulletin MANUFACTURER Raven Lining Systems 13105 E. 61 st Street, Suite A Broken Arrow, OK 74012 (918) 6150020 TENSILE TESTING OF PLASTICS ASTM D638, ISO 527 Tensile tests measure the force
More informationSUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES
SUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES T.R. Emery 1, J. M. DulieuBarton 1, P.R. Cunningham 2 1 University of Southampton, School of Engineering Sciences, SO17 1BJ, UK
More informationMassachusetts Institute of Technology Department of Mechanical Engineering Cambridge, MA 02139
Massachusetts Institute of Technology Department of Mechanical Engineering Cambridge, MA 02139 2.002 Mechanics and Materials II Spring 2004 Laboratory Module No. 6 Fracture Toughness Testing and Residual
More informationInsitu local strain measurement in textile composites with embedded optical fibre sensors
Insitu local strain measurement in textile composites with embedded optical fibre sensors S. Daggumati, E. Voet, I. De Baere, W. Van Paepegem & J. Degrieck Ghent University, Department of Materials Science
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationDEFLECTION OF BEAMS WlTH SPECIAL REFERENCE TO SHEAR DEFORMATIONS
DEFLECTION OF BEAMS WlTH SPECIAL REFERENCE TO SHEAR DEFORMATIONS THE INFLUENCE OF THE FORM OF A WOODEN BEAM ON ITS STIFFNESS AND STRENGTHI (REPRINT FROM NATIONAL ADVISORY COMMITTEE FOR AERONAUTICS REPORT
More informationEVALUATION OF DEBONDING ENERGY RELEASE RATE OF EXTERNALLY BONDED FRP SHEETS FOR REHABILITATION OF INFRASTRUCTURES
EVALUATION OF DEBONDING ENERGY RELEASE RATE OF EXTERNALLY BONDED FRP SHEETS FOR REHABILITATION OF INFRASTRUCTURES Koji YAMAGUCHI 1, Isao KIMPARA 1, and Kazuro KAGEYAMA 1 1 Department of Environmental &
More information16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS
6 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FRACTURE INTERFACE ELEMENTS FOR STATIC AND FATIUE ANALYSIS erald E. Mabson*, Lyle R. Deobald*, Bernhard Dopker*, D.M. Hoyt**, Jeffrey S. Baylor**, Douglas
More informationDETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1
PERIODICA POLYTECHNICA SER. CIV. ENG. VOL. 46, NO. 1, PP. 125 148 (2002) DETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1 Nándor LIEGNER Department of Highway and Railway Engineering
More informationDesign of a fastener based on negative Poisson's ratio foam adapted from
1 Design of a fastener based on negative Poisson's ratio foam adapted from Choi, J. B. and Lakes, R. S., "Design of a fastener based on negative Poisson's ratio foam", Cellular Polymers, 10, 205212 (1991).
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationUC San Diego UC San Diego Electronic Theses and Dissertations
UC San Diego UC San Diego Electronic Theses and Dissertations Title Low Velocity Impacts of Variable Tip Radius on Carbon/ Epoxy Plates / Permalink https://escholarship.org/uc/item/6q32d5q5 Author Delaney,
More information*Corresponding author: Keywords: Finiteelement analysis; Multiscale modelling; Onset theory; Dilatational strain invariant.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
More informationNonlinear Buckling Prediction in ANSYS. August 2009
Nonlinear Buckling Prediction in ANSYS August 2009 Buckling Overview Prediction of buckling of engineering structures is a challenging problem for several reasons: A real structure contains imperfections
More informationUsing ABAQUS Cohesive Elements to Model Peeling of an Epoxybonded Aluminum Strip: A Benchmark Study for Inelastic Peel Arms
Using ABAQUS Cohesive Elements to Model Peeling of an Epoxybonded Aluminum Strip: A Benchmark Study for Inelastic Peel Arms Ted Diehl DuPont DuPont Engineering Technology, Chestnut Run, Bldg 722, Wilmington,
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More information7.4 The Elementary Beam Theory
7.4 The Elementary Beam Theory In this section, problems involving long and slender beams are addressed. s with pressure vessels, the geometry of the beam, and the specific type of loading which will be
More informationFlexure: Behavior and Nominal Strength of Beam Sections
4 5000 4000 (increased d ) (increased f (increased A s or f y ) c or b) Flexure: Behavior and Nominal Strength of Beam Sections Moment (kipin.) 3000 2000 1000 0 0 (basic) (A s 0.5A s ) 0.0005 0.001 0.0015
More information4.MECHANICAL PROPERTIES OF MATERIALS
4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stressstrain diagram
More informationComposite Materials 261 and 262
Composite Materials 261 and 262 Stefan Hartmann 1 David Moncayo 2 1 DYNAmore GmbH, Stuttgart, Germany 2 Daimler AG, Sindelfingen, Germany 11. LSDYNA Forum 2012, 9.  10. Oktober 2012, Ulm 1 Outline Introduction
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationCEE575  Homework 1. Resistive Sensing: Due Monday, January 29
CEE575  Homework 1 Resistive Sensing: Due Monday, January 29 Problem 1: Planes A metallic wire embedded in a strain gage is 4 cm long with a diameter of 0.1 mm. The gage is mounted on the upper surface
More informationSHOCK FOCUSING IN WATER IN A CONVERGENT CARBON FIBER COMPOSITE STRUCTURE
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS SHOCK FOCUSING IN WATER IN A CONVERGENT CARBON FIBER COMPOSITE STRUCTURE C. Wang 1, V. Eliasson 2 * 1 Department of Physics, University of Southern
More informationTESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS
TESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS I. M. Daniel, J. L. Abot, and K. A. Wang Walter P. Murphy Professor, Departments of Civil and Mechanical Engineering, Robert R. McCormick School of Engineering
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More informationIMECE CRACK TUNNELING: EFFECT OF STRESS CONSTRAINT
Proceedings of IMECE04 2004 ASME International Mechanical Engineering Congress November 1320, 2004, Anaheim, California USA IMECE200460700 CRACK TUNNELING: EFFECT OF STRESS CONSTRAINT Jianzheng Zuo Department
More informationDEVELOPMENT OF DROP WEIGHT IMPACT TEST MACHINE
CHAPTER8 DEVELOPMENT OF DROP WEIGHT IMPACT TEST MACHINE 8.1 Introduction The behavior of materials is different when they are subjected to dynamic loading [9]. The testing of materials under dynamic conditions
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationUnified Quiz M4 May 7, 2008 M  PORTION
9:0010: 00 (last four digits) 32141 Unified Quiz M4 May 7, 2008 M  PORTION Put the last four digits of your MIT ID # on each page of the exam. Read all questions carefully. Do all work on that question
More informationTMHL TMHL (Del I, teori; 1 p.) SOLUTION I. II.. III. Fig. 1.1
TMHL6 2040830 (Del I, teori; p.). Fig.. shows three cases of sharp cracks in a sheet of metal. In all three cases, the sheet is assumed to be very large in comparison with the crack. Note the different
More informationNumerical modelling of contact for low velocity impact damage in composite laminates J. Bonini, F. Collombet, J.L. Lataillade
Numerical modelling of contact for low velocity impact damage in composite laminates J. Bonini, F. Collombet, J.L. Lataillade Esplanade des Arts et Metiers, INTRODUCTION A low velocity impact on a composite
More informationADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF COMPOSITES
NAFEMS WORLD CONGRESS 13, SALZBURG, AUSTRIA ADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF M. Bruyneel, J.P. Delsemme, P. Jetteur (LMS Samtech, Belgium); A.C. Goupil (ISMANS, France). Dr. Ir. M. Bruyneel,
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationSize Effects In the Crushing of Honeycomb Structures
45th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics & Materials Conference 1922 April 2004, Palm Springs, California AIAA 20041640 Size Effects In the Crushing of Honeycomb Structures Erik C.
More informationAfter lecture 16 you should be able to
Lecture 16: Design of paper and board packaging Advanced concepts: FEM, Fracture Mechanics After lecture 16 you should be able to describe the finite element method and its use for paper based industry
More informationAC829A. Issued on Apr. 15 th 2013 (Version 1.0)
Hitachi Chemical Co., Ltd. Hitachi Anisotropic Conductive Film ANISOLM AC829A Issued on Apr. 15 th 2013 (Version 1.0) 1. Standard specification, bonding condition, storage condition and characteristic.....1
More informationFINITE ELEMENT MODELING OF DELAMINATION DAMAGE IN CARBON FIBER LAMINATES SUBJECT TO LOWVELOCITY IMPACT AND
FINITE ELEMENT MODELING OF DELAMINATION DAMAGE IN CARBON FIBER LAMINATES SUBJECT TO LOWVELOCITY IMPACT AND COMPARISON WITH EXPERIMENTAL IMPACT TESTS USING NONDESTRUCTIVE VIBROTHERMOGRAPHY EVALUATION A
More informationBRIDGED DELAMINATION CRACKS IN CURVED BEAMS AND MIXEDMODE BENDING SPECIMENS
BRDGED DELANATON CRACKS N CURVED BEAS AND XEDODE BENDNG SPECENS Roberta assabò and Brian N. Cox Department of Structural and Geotechnical Engineering, University of Genova, Via ontallegro, 645, Genova,
More informationEXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS
EXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS Kevin L. Peil +, Ever J. Barbero +, Eduardo M. Sosa* + Department of Mechanical and Aerospace Engineering, West Virginia University (WVU), Morgantown,
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationMULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS
MULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS F.X. Irisarri, J.F. Maire* and N. Carrere ONERA, 9 av. de la Division Leclerc, 930 Châtillon, France francoisxavier.irisarri@onera.fr,
More informationTable of Contents. iii
Table of Contents Foreword..................................................... xv Preface...................................................... xvii Acknowledgements.............................................
More informationDegree Thesis Flexural Rigidity (D) in Beams. Author: Zious Karis. Instructor: Rene Herrmann
Degree Thesis Flexural Rigidity (D) in Beams Author: Zious Karis Instructor: Rene Herrmann Degree Thesis Materials Processing Technology 2017 DEGREE THESIS Arcada University of Applied Sciences, Helsinki,
More informationDon Robbins, Andrew Morrison, Rick Dalgarno Autodesk, Inc., Laramie, Wyoming. Abstract
PROGRESSIVE FAILURE SIMULATION OF ASMANUFACTURED SHORT FIBER FILLED INJECTION MOLDED PARTS: VALIDATION FOR COMPLEX GEOMETRIES AND COMBINED LOAD CONDITIONS Don Robbins, Andrew Morrison, Rick Dalgarno Autodesk,
More informationNonLinear Finite Element Modeling of THUNDER Piezoelectric Actuators
NonLinear Finite Element Modeling of THUNDER Piezoelectric Actuators Barmac K. Taleghani 1, Joel F. Campbell 2 1 Army Research Laboratory, Vehicle Technology Center, MS 230 NASA Langley Research Center,
More informationPoisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics
10.1111/j.14602695.2007.01095.x Poisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics W. VAN PAEPEGEM, I. DE BAERE, E. LAMKANFI and J. DEGRIECK Ghent University, Department
More informationEquipotential Lines and Electric Fields
Physics Equipotential Lines and Electric Fields Plotting the Electric Field MATERIALS AND RESOURCES EACH GROUP 5 alligator clip leads 2 batteries, 9 V 2 binder clips, large computer LabQuest multimeter,
More informationFailure Mode Predictions in the Compressive Response of Laminated Composites
Structures, Structural Dynamics, and Materials and Colocated Conferences April 811, 2013, Boston, Massachusetts 54th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference AIAA
More informationDTU Space Carbon Fiber Reinforced Plastic and CFRP projects. Niels Christian Jessen Hans Ulrik NørgaardNielsen
DTU Space Carbon Fiber Reinforced Plastic and CFRP projects Niels Christian Jessen Hans Ulrik NørgaardNielsen Why CFRP + Material properties can be designed + High Specific Stiffness Young's module /
More informationDrilling of carbon fibre reinforced laminates a study
Drilling of carbon fibre reinforced laminates a study Luís M. P. Durão 1a, Daniel J. S. Gonçalves 1b, João Manuel R. S. Tavares 2c, Victor H. C. Albuquerque 2c, A. Torres Marques 2c, A. M. Baptista 2c
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationValidity of fracture mechanics concepts applied to wood by finite element calculation
Wood Sci. Technol. 18:5158 (1984) Wood Science and Technology 9 SpringerVerlag 1984 Validity of fracture mechanics concepts applied to wood by finite element calculation P. Triboulot*, Champenoux, P.
More informationPrinciples of Almen Strip Selection
academic study Prof. Dr. David Kirk Coventry University, U.K. Principles of Almen Strip Selection INTRODUCTION The guiding principles for Almen strip selection are thickness, variability and shape. Thickness
More informationINTRODUCTION TO PIEZO TRANSDUCERS
PIEZO SYSTEMS, INC. 65 Tower Office Park Woburn, MA 01801 USA Tel: 781 933 4850 Fax: 781 933 4743 email: sales@piezo.com Find Search for a product or category HOME PRODUCTS CUSTOM OEM CATALOG TECHNICAL
More informationStandard Test Methods for PlaneStrain Fracture Toughness and Strain Energy Release Rate of Plastic Materials 1
This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards,
More informationDelamination in fractured laminated glass
Delamination in fractured laminated glass Caroline BUTCHART*, Mauro OVEREND a * Department of Engineering, University of Cambridge Trumpington Street, Cambridge, CB2 1PZ, UK cvb25@cam.ac.uk a Department
More information